LMucko/crystallography-open-database huggingface dataset:
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1000, MoKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006222
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1000,
 MoKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0867
_cell_length_b                   8.0867
_cell_length_c                   8.0867
_cell_formula_units_Z            8
_cell_volume                     528.827
_database_code_amcsd             0007804
_exptl_crystal_density_diffrn    4.606
_cod_original_cell_volume        528.828
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006222
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1100, MoKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006223
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1100,
 MoKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0871
_cell_length_b                   8.0871
_cell_length_c                   8.0871
_cell_formula_units_Z            8
_cell_volume                     528.906
_database_code_amcsd             0007805
_exptl_crystal_density_diffrn    4.605
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006223
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1200, MoKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006224
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1200,
 MoKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0876
_cell_length_b                   8.0876
_cell_length_c                   8.0876
_cell_formula_units_Z            8
_cell_volume                     529.004
_database_code_amcsd             0007806
_exptl_crystal_density_diffrn    4.604
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006224
_cod_duplicate_entry 9006209
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1300, MoKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006225
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1300,
 MoKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0884
_cell_length_b                   8.0884
_cell_length_c                   8.0884
_cell_formula_units_Z            8
_cell_volume                     529.161
_database_code_amcsd             0007807
_exptl_crystal_density_diffrn    4.603
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006225
_cod_duplicate_entry 9006210
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/900, CuKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006226
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/900,
 CuKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0865
_cell_length_b                   8.0865
_cell_length_c                   8.0865
_cell_formula_units_Z            8
_cell_volume                     528.788
_database_code_amcsd             0007808
_exptl_crystal_density_diffrn    4.606
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006226
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1000, CuKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006227
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1000,
 CuKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0867
_cell_length_b                   8.0867
_cell_length_c                   8.0867
_cell_formula_units_Z            8
_cell_volume                     528.827
_database_code_amcsd             0007809
_exptl_crystal_density_diffrn    4.606
_cod_original_cell_volume        528.828
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006227
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1100, CuKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006228
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1100,
 CuKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0871
_cell_length_b                   8.0871
_cell_length_c                   8.0871
_cell_formula_units_Z            8
_cell_volume                     528.906
_database_code_amcsd             0007810
_exptl_crystal_density_diffrn    4.605
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006228
_cod_duplicate_entry 9006208
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1200, CuKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006229
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1200,
 CuKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0876
_cell_length_b                   8.0876
_cell_length_c                   8.0876
_cell_formula_units_Z            8
_cell_volume                     529.004
_database_code_amcsd             0007811
_exptl_crystal_density_diffrn    4.604
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006229
_cod_duplicate_entry 9006214
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1300, CuKalpha1 radiation
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006230
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnAl2O4/1300,
 CuKalpha1 radiation
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Al2 O4 Zn'
_chemical_name_mineral           Gahnite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0884
_cell_length_b                   8.0884
_cell_length_c                   8.0884
_cell_formula_units_Z            8
_cell_volume                     529.161
_database_code_amcsd             0007812
_exptl_crystal_density_diffrn    4.603
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Al2 O4'
_cod_database_code               9006230
_cod_duplicate_entry 9006210
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/900, BGI (Mo radiation)
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006231
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/900, BGI (Mo
 radiation)
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Cr2 Mg O4'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3341
_cell_length_b                   8.3341
_cell_length_c                   8.3341
_cell_formula_units_Z            8
_cell_volume                     578.863
_database_code_amcsd             0007813
_exptl_crystal_density_diffrn    4.413
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Mg Cr2 O4'
_cod_database_code               9006231
_cod_duplicate_entry 9006185
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/1100, BGI (Mo radiation)
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006232
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/1100, BGI
 (Mo radiation)
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Cr2 Mg O4'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3342
_cell_length_b                   8.3342
_cell_length_c                   8.3342
_cell_formula_units_Z            8
_cell_volume                     578.884
_database_code_amcsd             0007814
_exptl_crystal_density_diffrn    4.413
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Mg Cr2 O4'
_cod_database_code               9006232
_cod_duplicate_entry 9006186
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/1300, BGI (Mo radiation)
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006233
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/1300, BGI
 (Mo radiation)
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Cr2 Mg O4'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3339
_cell_length_b                   8.3339
_cell_length_c                   8.3339
_cell_formula_units_Z            8
_cell_volume                     578.822
_database_code_amcsd             0007815
_exptl_crystal_density_diffrn    4.413
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Mg Cr2 O4'
_cod_database_code               9006233
_cod_duplicate_entry 9006187
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: ZnCr2O4, BGI (Mo radiation)
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006234
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: ZnCr2O4, BGI (Mo
 radiation)
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Cr2 O4 Zn'
_chemical_name_mineral           Zincochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3271
_cell_length_b                   8.3271
_cell_length_c                   8.3271
_cell_formula_units_Z            8
_cell_volume                     577.406
_database_code_amcsd             0007816
_exptl_crystal_density_diffrn    5.369
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Zn Cr2 O4'
_cod_database_code               9006234
_cod_duplicate_entry 9006220
Crystal structures and cation distributions in simple spinels from powder XRD structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/900, UCLA (Cu radiation)
O'Neill H St C; Dollase, W. A.; Physics and Chemistry of Minerals 20 (1994) 541–555; doi:10.1007/BF00211850

data_9006235
_publ_section_title
;Crystal structures and cation distributions in simple spinels from powder XRD
 structural refinements: MgCr2O4, ZnCr2O4, Fe3O4 and the temperature
 dependence of the cation distribution in ZnAl2O4 Sample: MgCr2O4/900, UCLA
 (Cu radiation)
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              541
_journal_page_last               555
_journal_paper_doi               10.1007/BF00211850
_journal_volume                  20
_journal_year                    1994
_chemical_formula_sum            'Cr2 Mg O4'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3341
_cell_length_b                   8.3341
_cell_length_c                   8.3341
_cell_formula_units_Z            8
_cell_volume                     578.863
_database_code_amcsd             0007817
_exptl_crystal_density_diffrn    4.413
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Mg Cr2 O4'
_cod_database_code               9006235
_cod_duplicate_entry 9006180